#------------------------------------------------------------------------------
#$Date: 2020-10-04 06:19:33 +0300 (Sun, 04 Oct 2020) $
#$Revision: 257094 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/51/74/4517486.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4517486
loop_
_publ_author_name
'Yang, Xiya'
'Sha, Jingquan'
'Li, Wenjing'
'Tan, Zenglong'
'Hou, Liran'
'Jiang, Jianzhuang'
_publ_section_title
;
 Ternary Cross-Vanadium Tetra-Capped POMOFs@PPy/RGO Nanocomposites with
 Hybrid Battery-Supercapacitor Behavior for Enhancing Lithium Battery
 Storage
;
_journal_issue                   11
_journal_name_full               'ACS Sustainable Chemistry & Engineering'
_journal_page_first              4667
_journal_page_last               4675
_journal_paper_doi               10.1021/acssuschemeng.0c01162
_journal_volume                  8
_journal_year                    2020
_chemical_formula_moiety         'C16 H16 Cl Cu12 Mo12 N24 O47 P V3'
_chemical_formula_sum            'C16 H16 Cl Cu12 Mo12 N24 O47 P V3'
_chemical_formula_weight         3429.65
_space_group_crystal_system      monoclinic
_space_group_IT_number           12
_space_group_name_Hall           '-C 2y'
_space_group_name_H-M_alt        'C 1 2/m 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 120.954(2)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   17.261(2)
_cell_length_b                   14.564(2)
_cell_length_c                   14.563(3)
_cell_measurement_reflns_used    7982
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      25.000
_cell_measurement_theta_min      1.962
_cell_volume                     3139.6(9)
_computing_cell_refinement       'Bruker XSCANS'
_computing_data_collection       'Bruker XSCANS'
_computing_data_reduction        'Bruker SHELXTL'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'Bruker SHELXTL'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Bruker P4'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0182
_diffrn_reflns_av_unetI/netI     0.0211
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -18
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            7982
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.000
_diffrn_reflns_theta_max         25.000
_diffrn_reflns_theta_min         1.962
_diffrn_source                   'sealed tube'
_exptl_absorpt_coefficient_mu    6.882
_exptl_absorpt_correction_T_max  0.179
_exptl_absorpt_correction_T_min  0.051
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Sheldrick,1996)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    3.628
_exptl_crystal_description       block
_exptl_crystal_F_000             3218
_exptl_crystal_size_max          0.7
_exptl_crystal_size_mid          0.4
_exptl_crystal_size_min          0.25
_refine_diff_density_max         3.216
_refine_diff_density_min         -2.972
_refine_diff_density_rms         0.311
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.064
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     281
_refine_ls_number_reflns         2893
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.064
_refine_ls_R_factor_all          0.0710
_refine_ls_R_factor_gt           0.0642
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.1181P)²+135.8597P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1966
_refine_ls_wR_factor_ref         0.2029
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2523
_reflns_number_total             2899
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            sc0c01162_si_002.cif
_cod_data_source_block           1
_cod_depositor_comments
;Adding full bibliography for 4517486--4517487.cif.

 Adding full bibliography for 4517486--4517487.cif.
;
_cod_original_sg_symbol_H-M      'C 2/m'
_cod_database_code               4517486
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
C1 C 0.8590(8) 0.6859(8) -0.0121(9) 0.032(3) Uani 1 1 d . . . . .
H1 H 0.8438 0.6664 0.0376 0.038 Uiso 1 1 calc R U . . .
C2 C 0.8915(8) 0.6852(8) -0.1337(9) 0.029(2) Uani 1 1 d . . . . .
H2 H 0.9033 0.6653 -0.1860 0.035 Uiso 1 1 calc R U . . .
C3 C 1.0933(7) 0.0721(8) 0.3633(9) 0.025(2) Uani 1 1 d . . . . .
H3 H 1.0956 0.1328 0.3844 0.030 Uiso 1 1 calc R U . . .
C4 C 1.1401(8) -0.0719(9) 0.7669(10) 0.033(3) Uani 1 1 d . . . . .
H4 H 1.1404 -0.1325 0.7470 0.040 Uiso 1 1 calc R U . . .
N1 N 0.8931(6) 0.7729(7) -0.1074(7) 0.026(2) Uani 1 1 d . . . . .
N2 N 1.1411(6) -0.0476(7) 0.8557(7) 0.027(2) Uani 1 1 d . . . . .
N3 N 1.1386(10) 0.0000 0.7100(11) 0.033(3) Uani 1 2 d S T P . .
N4 N 0.8709(7) 0.6285(6) -0.0763(7) 0.027(2) Uani 1 1 d . . . . .
N5 N 1.0845(6) 0.0475(6) 0.2726(7) 0.0222(18) Uani 1 1 d . . . . .
N6 N 0.8711(6) 0.7730(7) -0.0274(7) 0.028(2) Uani 1 1 d . . . . .
N7 N 1.0986(9) 0.0000 0.4226(11) 0.025(3) Uani 1 2 d S T P . .
O1 O 0.7240(9) 0.5000 0.1068(10) 0.051(4) Uani 1 2 d S T P . .
O2 O 0.9740(7) 0.2489(6) 0.2312(7) 0.043(2) Uani 1 1 d . . . . .
O3 O 1.0644(7) 0.4108(6) 0.3123(7) 0.050(3) Uani 1 1 d . . . . .
O4 O 0.9059(7) 0.2802(8) 0.3649(8) 0.054(3) Uani 1 1 d . . . . .
O5 O 0.7472(7) 0.2514(7) 0.3754(9) 0.061(3) Uani 1 1 d . . . . .
O6 O 0.7972(8) 0.4096(8) 0.4903(8) 0.065(3) Uani 1 1 d . . . . .
O7 O 0.8897(8) 0.4111(8) 0.2250(9) 0.061(3) Uani 1 1 d . . . . .
O8 O 0.7751(9) 0.5921(10) 0.2940(11) 0.080(5) Uani 1 1 d . . . . .
O9 O 1.2234(12) 0.5000 0.3574(15) 0.074(5) Uani 1 2 d S T P . .
O11 O 0.9337(9) 0.4376(10) 0.4044(10) 0.073(3) Uani 1 1 d . . . . .
O12 O 1.0746(7) 0.2810(7) 0.4496(6) 0.044(2) Uani 1 1 d . . . . .
O10 O 1.0529(10) 0.4408(10) 0.4652(10) 0.078(4) Uani 1 1 d . . . . .
O13 O 0.984(4) 0.5000 0.106(4) 0.112(17) Uani 0.5 2 d S T P . .
P1 P 1.0000 0.5000 0.5000 0.0128(9) Uani 1 4 d S T P . .
Cu2 Cu 0.91503(11) 0.87767(11) -0.16628(13) 0.0376(4) Uani 1 1 d . . . . .
Cu3 Cu 0.87018(16) 0.5000 -0.07766(18) 0.0366(5) Uani 1 2 d S T P . .
Cu4 Cu 1.12049(18) 0.0000 0.56805(19) 0.0448(6) Uani 1 2 d S T P . .
Cu1 Cu 1.12975(12) -0.12295(12) 0.95277(13) 0.0426(5) Uani 1 1 d . . . . .
Cl1 Cl 1.0000 1.0000 0.0000 0.056(2) Uani 1 4 d S T P . .
V2 V 0.9825(7) 0.5000 0.2192(7) 0.066(2) Uani 0.5 2 d S T P . .
Mo1 Mo 0.98064(8) 0.33225(8) 0.31290(9) 0.0393(4) Uani 1 1 d . . . . .
Mo2 Mo 0.80939(11) 0.5000 0.23112(13) 0.0430(5) Uani 1 2 d S T P . .
Mo3 Mo 0.82425(8) 0.33203(8) 0.41261(9) 0.0415(4) Uani 1 1 d . . . . .
Mo4 Mo 1.15489(15) 0.5000 0.40455(18) 0.0549(6) Uani 1 2 d S T P . .
O15 O 1.0407 0.1106 0.5249 0.068(6) Uiso 0.5 1 d . . P . .
V1 V 1.0000 0.2279 0.5000 0.0640(12) Uani 1 2 d S T P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
N6 C1 N4 112.5(10) . . ?
N6 C1 H1 123.7 . . ?
N4 C1 H1 123.7 . . ?
N1 C2 N4 112.5(9) . . ?
N1 C2 H2 123.7 . . ?
N4 C2 H2 123.7 . . ?
N5 C3 N7 112.1(10) . . ?
N5 C3 H3 124.0 . . ?
N7 C3 H3 124.0 . . ?
N3 C4 N2 112.5(11) . . ?
N3 C4 H4 123.7 . . ?
N2 C4 H4 123.7 . . ?
C2 N1 N6 105.5(9) . . ?
C2 N1 Cu2 128.8(8) . . ?
N6 N1 Cu2 125.7(7) . . ?
C4 N2 N2 105.4(7) . 6 ?
C4 N2 Cu1 128.4(8) . . ?
N2 N2 Cu1 125.8(3) 6 . ?
C4 N3 C4 104.2(13) . 6 ?
C4 N3 Cu4 127.6(7) . . ?
C4 N3 Cu4 127.6(7) 6 . ?
C2 N4 C1 103.6(9) . . ?
C2 N4 Cu3 127.6(8) . . ?
C1 N4 Cu3 128.6(8) . . ?
C3 N5 N5 105.9(6) . 6 ?
C3 N5 Cu2 128.7(8) . 5_765 ?
N5 N5 Cu2 125.0(3) 6 5_765 ?
C1 N6 N1 105.9(9) . . ?
C1 N6 Cu1 129.0(8) . 2_766 ?
N1 N6 Cu1 124.9(7) . 2_766 ?
C3 N7 C3 104.0(13) . 6 ?
C3 N7 Cu4 127.9(6) . . ?
C3 N7 Cu4 127.9(6) 6 . ?
Mo1 O3 V2 97.5(5) . . ?
Mo1 O3 Mo4 139.8(6) . . ?
V2 O3 Mo4 94.3(5) . . ?
V1 O4 Mo1 99.7(4) . . ?
V1 O4 Mo3 99.5(4) . . ?
Mo1 O4 Mo3 135.0(6) . . ?
Mo3 O6 Mo4 143.4(8) . 5_766 ?
Mo1 O7 Mo2 139.9(6) . . ?
Mo1 O7 V2 91.0(5) . . ?
Mo2 O7 V2 99.8(5) . . ?
Mo3 O8 Mo2 140.5(8) 6_565 . ?
Mo4 O9 Cu4 135.5(10) . 7_756 ?
P1 O11 O10 53.7(6) . . ?
P1 O11 O10 53.4(6) . 2_756 ?
O10 O11 O10 89.2(9) . 2_756 ?
P1 O11 Mo1 124.0(7) . . ?
O10 O11 Mo1 70.2(6) . . ?
O10 O11 Mo1 134.5(9) 2_756 . ?
P1 O11 Mo3 123.0(6) . . ?
O10 O11 Mo3 135.0(8) . . ?
O10 O11 Mo3 69.7(6) 2_756 . ?
Mo1 O11 Mo3 96.4(5) . . ?
P1 O11 Mo2 123.0(7) . . ?
O10 O11 Mo2 131.9(8) . . ?
O10 O11 Mo2 129.6(8) 2_756 . ?
Mo1 O11 Mo2 91.8(4) . . ?
Mo3 O11 Mo2 89.7(4) . . ?
V1 O12 Mo1 100.0(4) . . ?
V1 O12 Mo3 100.1(4) . 2_756 ?
Mo1 O12 Mo3 135.7(5) . 2_756 ?
P1 O10 O10 55.4(5) . 6_565 ?
P1 O10 O11 55.9(6) . . ?
O10 O10 O11 91.5(7) 6_565 . ?
P1 O10 O11 55.5(6) . 2_756 ?
O10 O10 O11 91.5(7) 6_565 2_756 ?
O11 O10 O11 90.7(9) . 2_756 ?
P1 O10 Mo1 123.3(8) . . ?
O10 O10 Mo1 129.7(3) 6_565 . ?
O11 O10 Mo1 67.4(6) . . ?
O11 O10 Mo1 131.6(9) 2_756 . ?
P1 O10 Mo4 125.2(8) . . ?
O10 O10 Mo4 69.8(3) 6_565 . ?
O11 O10 Mo4 132.9(8) . . ?
O11 O10 Mo4 130.9(8) 2_756 . ?
Mo1 O10 Mo4 91.4(4) . . ?
P1 O10 Mo3 123.8(7) . 2_756 ?
O10 O10 Mo3 129.2(3) 6_565 2_756 ?
O11 O10 Mo3 132.7(9) . 2_756 ?
O11 O10 Mo3 68.3(6) 2_756 2_756 ?
Mo1 O10 Mo3 94.8(5) . 2_756 ?
Mo4 O10 Mo3 88.6(5) . 2_756 ?
V2 O13 Cu3 134(3) . . ?
O10 P1 O10 180.0(12) 6_565 2_756 ?
O10 P1 O10 110.9(10) 6_565 5_766 ?
O10 P1 O10 69.1(10) 2_756 5_766 ?
O10 P1 O10 69.1(10) 6_565 . ?
O10 P1 O10 110.9(10) 2_756 . ?
O10 P1 O10 180.0 5_766 . ?
O10 P1 O11 108.9(7) 6_565 . ?
O10 P1 O11 71.1(7) 2_756 . ?
O10 P1 O11 109.7(7) 5_766 . ?
O10 P1 O11 70.3(7) . . ?
O10 P1 O11 71.1(7) 6_565 5_766 ?
O10 P1 O11 108.9(7) 2_756 5_766 ?
O10 P1 O11 70.3(7) 5_766 5_766 ?
O10 P1 O11 109.7(7) . 5_766 ?
O11 P1 O11 180.0 . 5_766 ?
O10 P1 O11 70.3(7) 6_565 6_565 ?
O10 P1 O11 109.7(7) 2_756 6_565 ?
O10 P1 O11 71.1(7) 5_766 6_565 ?
O10 P1 O11 108.9(7) . 6_565 ?
O11 P1 O11 71.3(10) . 6_565 ?
O11 P1 O11 108.7(10) 5_766 6_565 ?
O10 P1 O11 109.7(7) 6_565 2_756 ?
O10 P1 O11 70.3(7) 2_756 2_756 ?
O10 P1 O11 108.9(7) 5_766 2_756 ?
O10 P1 O11 71.1(7) . 2_756 ?
O11 P1 O11 108.7(10) . 2_756 ?
O11 P1 O11 71.3(10) 5_766 2_756 ?
O11 P1 O11 180.0 6_565 2_756 ?
N1 Cu2 N5 157.5(4) . 5_765 ?
N1 Cu2 Cl1 105.4(3) . . ?
N5 Cu2 Cl1 97.1(3) 5_765 . ?
N4 Cu3 N4 179.0(6) . 6_565 ?
N4 Cu3 O13 89.5(3) . . ?
N4 Cu3 O13 89.5(3) 6_565 . ?
N3 Cu4 N7 178.4(6) . . ?
N3 Cu4 O15 92.4(3) . . ?
N7 Cu4 O15 86.6(2) . . ?
N3 Cu4 O15 92.4(3) . 6 ?
N7 Cu4 O15 86.6(2) . 6 ?
O15 Cu4 O15 107.38(13) . 6 ?
N3 Cu4 O9 89.4(6) . 7_756 ?
N7 Cu4 O9 92.2(6) . 7_756 ?
O15 Cu4 O9 126.23(7) . 7_756 ?
O15 Cu4 O9 126.23(6) 6 7_756 ?
N6 Cu1 N2 161.2(4) 2_746 . ?
Cu2 Cl1 Cu2 180.0 . 5_775 ?
Cu2 Cl1 Cu2 80.93(6) . 6_575 ?
Cu2 Cl1 Cu2 99.06(6) 5_775 6_575 ?
Cu2 Cl1 Cu2 99.07(6) . 2_755 ?
Cu2 Cl1 Cu2 80.94(6) 5_775 2_755 ?
Cu2 Cl1 Cu2 180.00(5) 6_575 2_755 ?
O13 V2 O3 109.0(15) . . ?
O13 V2 O3 109.0(15) . 6_565 ?
O3 V2 O3 87.1(7) . 6_565 ?
O13 V2 O7 116.2(16) . . ?
O3 V2 O7 81.4(4) . . ?
O3 V2 O7 134.6(7) 6_565 . ?
O13 V2 O7 116.2(16) . 6_565 ?
O3 V2 O7 134.6(7) . 6_565 ?
O3 V2 O7 81.4(4) 6_565 6_565 ?
O7 V2 O7 76.3(6) . 6_565 ?
O13 V2 Mo4 114(2) . . ?
O3 V2 Mo4 43.6(3) . . ?
O3 V2 Mo4 43.6(3) 6_565 . ?
O7 V2 Mo4 114.5(4) . . ?
O7 V2 Mo4 114.5(4) 6_565 . ?
O13 V2 Mo1 119.50(16) . . ?
O3 V2 Mo1 40.7(3) . . ?
O3 V2 Mo1 116.2(5) 6_565 . ?
O7 V2 Mo1 40.7(3) . . ?
O7 V2 Mo1 108.5(5) 6_565 . ?
Mo4 V2 Mo1 78.7(2) . . ?
O13 V2 Mo1 119.50(16) . 6_565 ?
O3 V2 Mo1 116.2(5) . 6_565 ?
O3 V2 Mo1 40.7(3) 6_565 6_565 ?
O7 V2 Mo1 108.5(5) . 6_565 ?
O7 V2 Mo1 40.7(3) 6_565 6_565 ?
Mo4 V2 Mo1 78.7(2) . 6_565 ?
Mo1 V2 Mo1 121.0(3) . 6_565 ?
O13 V2 Mo2 124(2) . . ?
O3 V2 Mo2 110.4(5) . . ?
O3 V2 Mo2 110.4(5) 6_565 . ?
O7 V2 Mo2 38.2(3) . . ?
O7 V2 Mo2 38.2(3) 6_565 . ?
Mo4 V2 Mo2 121.6(3) . . ?
Mo1 V2 Mo2 73.6(2) . . ?
Mo1 V2 Mo2 73.6(2) 6_565 . ?
O2 Mo1 O7 103.8(5) . . ?
O2 Mo1 O3 102.4(5) . . ?
O7 Mo1 O3 90.0(5) . . ?
O2 Mo1 O4 100.2(5) . . ?
O7 Mo1 O4 90.9(4) . . ?
O3 Mo1 O4 156.5(5) . . ?
O2 Mo1 O12 99.6(5) . . ?
O7 Mo1 O12 156.1(5) . . ?
O3 Mo1 O12 90.0(4) . . ?
O4 Mo1 O12 79.9(4) . . ?
O2 Mo1 O11 159.2(5) . . ?
O7 Mo1 O11 65.2(5) . . ?
O3 Mo1 O11 95.4(5) . . ?
O4 Mo1 O11 63.9(5) . . ?
O12 Mo1 O11 91.0(4) . . ?
O2 Mo1 O10 157.7(5) . . ?
O7 Mo1 O10 94.7(5) . . ?
O3 Mo1 O10 64.8(5) . . ?
O4 Mo1 O10 91.7(5) . . ?
O12 Mo1 O10 63.9(4) . . ?
O11 Mo1 O10 42.4(5) . . ?
O2 Mo1 V2 107.5(3) . . ?
O7 Mo1 V2 48.2(4) . . ?
O3 Mo1 V2 41.8(4) . . ?
O4 Mo1 V2 134.5(4) . . ?
O12 Mo1 V2 128.0(3) . . ?
O11 Mo1 V2 78.9(4) . . ?
O10 Mo1 V2 75.7(4) . . ?
O2 Mo1 V1 102.5(3) . . ?
O7 Mo1 V1 127.7(3) . . ?
O3 Mo1 V1 126.8(3) . . ?
O4 Mo1 V1 40.1(3) . . ?
O12 Mo1 V1 39.8(3) . . ?
O11 Mo1 V1 74.5(3) . . ?
O10 Mo1 V1 74.9(3) . . ?
V2 Mo1 V1 149.69(17) . . ?
O1 Mo2 O8 102.0(6) . . ?
O1 Mo2 O8 102.0(6) . 6_565 ?
O8 Mo2 O8 90.8(8) . 6_565 ?
O1 Mo2 O7 102.0(5) . 6_565 ?
O8 Mo2 O7 87.6(5) . 6_565 ?
O8 Mo2 O7 155.8(6) 6_565 6_565 ?
O1 Mo2 O7 102.0(5) . . ?
O8 Mo2 O7 155.8(6) . . ?
O8 Mo2 O7 87.6(4) 6_565 . ?
O7 Mo2 O7 84.1(7) 6_565 . ?
O1 Mo2 O11 158.5(3) . . ?
O8 Mo2 O11 95.1(6) . . ?
O8 Mo2 O11 64.6(5) 6_565 . ?
O7 Mo2 O11 91.5(5) 6_565 . ?
O7 Mo2 O11 62.5(4) . . ?
O1 Mo2 O11 158.5(3) . 6_565 ?
O8 Mo2 O11 64.6(5) . 6_565 ?
O8 Mo2 O11 95.1(6) 6_565 6_565 ?
O7 Mo2 O11 62.5(4) 6_565 6_565 ?
O7 Mo2 O11 91.5(5) . 6_565 ?
O11 Mo2 O11 42.7(7) . 6_565 ?
O1 Mo2 V2 106.5(5) . . ?
O8 Mo2 V2 125.8(3) . . ?
O8 Mo2 V2 125.8(3) 6_565 . ?
O7 Mo2 V2 42.0(3) 6_565 . ?
O7 Mo2 V2 42.0(3) . . ?
O11 Mo2 V2 72.7(3) . . ?
O11 Mo2 V2 72.7(3) 6_565 . ?
O5 Mo3 O6 103.0(6) . . ?
O5 Mo3 O8 102.4(6) . 6_565 ?
O6 Mo3 O8 93.9(6) . 6_565 ?
O5 Mo3 O12 101.9(5) . 2_756 ?
O6 Mo3 O12 88.8(4) . 2_756 ?
O8 Mo3 O12 154.3(5) 6_565 2_756 ?
O5 Mo3 O4 102.1(6) . . ?
O6 Mo3 O4 153.7(5) . . ?
O8 Mo3 O4 88.2(4) 6_565 . ?
O12 Mo3 O4 78.6(4) 2_756 . ?
O5 Mo3 O11 158.8(5) . . ?
O6 Mo3 O11 95.2(5) . . ?
O8 Mo3 O11 65.2(5) 6_565 . ?
O12 Mo3 O11 89.1(4) 2_756 . ?
O4 Mo3 O11 62.0(5) . . ?
O5 Mo3 O10 158.6(5) . 2_756 ?
O6 Mo3 O10 64.0(5) . 2_756 ?
O8 Mo3 O10 95.7(6) 6_565 2_756 ?
O12 Mo3 O10 62.7(4) 2_756 2_756 ?
O4 Mo3 O10 89.7(5) . 2_756 ?
O11 Mo3 O10 42.0(4) . 2_756 ?
O5 Mo3 V1 104.3(4) . . ?
O6 Mo3 V1 124.9(3) . . ?
O8 Mo3 V1 124.9(3) 6_565 . ?
O12 Mo3 V1 39.2(3) 2_756 . ?
O4 Mo3 V1 39.5(3) . . ?
O11 Mo3 V1 73.0(3) . . ?
O10 Mo3 V1 73.7(3) 2_756 . ?
O9 Mo4 O6 103.5(6) . 5_766 ?
O9 Mo4 O6 103.5(6) . 2_756 ?
O6 Mo4 O6 90.1(8) 5_766 2_756 ?
O9 Mo4 O3 101.9(6) . . ?
O6 Mo4 O3 154.4(6) 5_766 . ?
O6 Mo4 O3 87.4(4) 2_756 . ?
O9 Mo4 O3 101.9(6) . 6_565 ?
O6 Mo4 O3 87.4(4) 5_766 6_565 ?
O6 Mo4 O3 154.4(6) 2_756 6_565 ?
O3 Mo4 O3 84.0(6) . 6_565 ?
O9 Mo4 O10 159.7(3) . . ?
O6 Mo4 O10 92.8(5) 5_766 . ?
O6 Mo4 O10 63.9(5) 2_756 . ?
O3 Mo4 O10 63.3(4) . . ?
O3 Mo4 O10 90.8(5) 6_565 . ?
O9 Mo4 O10 159.7(3) . 6_565 ?
O6 Mo4 O10 63.9(5) 5_766 6_565 ?
O6 Mo4 O10 92.8(5) 2_756 6_565 ?
O3 Mo4 O10 90.8(5) . 6_565 ?
O3 Mo4 O10 63.3(4) 6_565 6_565 ?
O10 Mo4 O10 40.4(7) . 6_565 ?
O9 Mo4 V2 103.4(7) . . ?
O6 Mo4 V2 126.5(3) 5_766 . ?
O6 Mo4 V2 126.5(3) 2_756 . ?
O3 Mo4 V2 42.1(3) . . ?
O3 Mo4 V2 42.1(3) 6_565 . ?
O10 Mo4 V2 75.5(4) . . ?
O10 Mo4 V2 75.5(4) 6_565 . ?
O15 O15 V1 70.573(3) 2_756 . ?
O15 O15 Cu4 126.21(6) 2_756 . ?
V1 O15 Cu4 163.02(6) . . ?
O15 V1 O15 38.848(7) 2_756 . ?
O15 V1 O12 100.8(3) 2_756 2_756 ?
O15 V1 O12 124.4(3) . 2_756 ?
O15 V1 O12 124.4(3) 2_756 . ?
O15 V1 O12 100.8(3) . . ?
O12 V1 O12 133.0(6) 2_756 . ?
O15 V1 O4 127.3(4) 2_756 2_756 ?
O15 V1 O4 97.5(4) . 2_756 ?
O12 V1 O4 80.4(4) 2_756 2_756 ?
O12 V1 O4 81.7(4) . 2_756 ?
O15 V1 O4 97.5(4) 2_756 . ?
O15 V1 O4 127.3(4) . . ?
O12 V1 O4 81.7(4) 2_756 . ?
O12 V1 O4 80.4(4) . . ?
O4 V1 O4 134.0(8) 2_756 . ?
O15 V1 Mo1 116.59(2) 2_756 . ?
O15 V1 Mo1 120.85(2) . . ?
O12 V1 Mo1 110.9(3) 2_756 . ?
O12 V1 Mo1 40.2(3) . . ?
O4 V1 Mo1 111.5(3) 2_756 . ?
O4 V1 Mo1 40.2(3) . . ?
O15 V1 Mo1 120.85(2) 2_756 2_756 ?
O15 V1 Mo1 116.59(2) . 2_756 ?
O12 V1 Mo1 40.2(3) 2_756 2_756 ?
O12 V1 Mo1 110.9(3) . 2_756 ?
O4 V1 Mo1 40.2(3) 2_756 2_756 ?
O4 V1 Mo1 111.5(3) . 2_756 ?
Mo1 V1 Mo1 118.78(4) . 2_756 ?
O15 V1 Mo3 139.35(2) 2_756 2_756 ?
O15 V1 Mo3 100.77(2) . 2_756 ?
O12 V1 Mo3 111.0(3) 2_756 2_756 ?
O12 V1 Mo3 40.7(3) . 2_756 ?
O4 V1 Mo3 41.0(3) 2_756 2_756 ?
O4 V1 Mo3 111.3(3) . 2_756 ?
Mo1 V1 Mo3 75.28(3) . 2_756 ?
Mo1 V1 Mo3 75.14(3) 2_756 2_756 ?
O15 V1 Mo3 100.77(2) 2_756 . ?
O15 V1 Mo3 139.35(2) . . ?
O12 V1 Mo3 40.7(3) 2_756 . ?
O12 V1 Mo3 111.0(3) . . ?
O4 V1 Mo3 111.3(3) 2_756 . ?
O4 V1 Mo3 41.0(3) . . ?
Mo1 V1 Mo3 75.14(3) . . ?
Mo1 V1 Mo3 75.28(3) 2_756 . ?
Mo3 V1 Mo3 119.83(4) 2_756 . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
C1 N6 1.324(15) . ?
C1 N4 1.347(15) . ?
C1 H1 0.9300 . ?
C2 N1 1.330(15) . ?
C2 N4 1.346(15) . ?
C2 H2 0.9300 . ?
C3 N5 1.300(14) . ?
C3 N7 1.332(13) . ?
C3 H3 0.9300 . ?
C4 N3 1.328(15) . ?
C4 N2 1.333(14) . ?
C4 H4 0.9300 . ?
N1 N6 1.399(13) . ?
N1 Cu2 1.881(9) . ?
N2 N2 1.39(2) 6 ?
N2 Cu1 1.877(9) . ?
N3 C4 1.328(15) 6 ?
N3 Cu4 1.925(13) . ?
N4 Cu3 1.872(9) . ?
N5 N5 1.385(17) 6 ?
N5 Cu2 1.897(9) 5_765 ?
N6 Cu1 1.869(9) 2_766 ?
N7 C3 1.332(13) 6 ?
N7 Cu4 1.950(13) . ?
O1 Mo2 1.644(13) . ?
O2 Mo1 1.662(8) . ?
O3 Mo1 1.847(9) . ?
O3 V2 1.885(11) . ?
O3 Mo4 1.942(9) . ?
O4 V1 1.950(9) . ?
O4 Mo1 1.954(9) . ?
O4 Mo3 2.012(9) . ?
O5 Mo3 1.643(9) . ?
O6 Mo3 1.822(10) . ?
O6 Mo4 1.860(10) 5_766 ?
O7 Mo1 1.831(10) . ?
O7 Mo2 1.932(10) . ?
O7 V2 2.094(14) . ?
O8 Mo3 1.848(10) 6_565 ?
O8 Mo2 1.884(11) . ?
O9 Mo4 1.644(14) . ?
O9 Cu4 2.331(18) 7_756 ?
O11 P1 1.561(14) . ?
O11 O10 1.77(2) . ?
O11 O10 1.790(18) 2_756 ?
O11 Mo1 2.429(13) . ?
O11 Mo3 2.485(14) . ?
O11 Mo2 2.496(13) . ?
O12 V1 1.940(9) . ?
O12 Mo1 1.957(8) . ?
O12 Mo3 2.006(9) 2_756 ?
O10 P1 1.519(14) . ?
O10 O10 1.72(3) 6_565 ?
O10 O11 1.790(18) 2_756 ?
O10 Mo1 2.476(14) . ?
O10 Mo4 2.495(14) . ?
O10 Mo3 2.508(14) 2_756 ?
O13 V2 1.66(4) . ?
O13 Cu3 2.37(5) . ?
P1 O10 1.519(14) 6_565 ?
P1 O10 1.519(14) 2_756 ?
P1 O10 1.519(14) 5_766 ?
P1 O11 1.561(14) 5_766 ?
P1 O11 1.561(14) 6_565 ?
P1 O11 1.561(14) 2_756 ?
Cu2 N5 1.897(9) 5_765 ?
Cu2 Cl1 2.7451(18) . ?
Cu3 N4 1.872(9) 6_565 ?
Cu4 O15 1.9990(16) . ?
Cu4 O15 1.9991(16) 6 ?
Cu4 O9 2.331(18) 7_756 ?
Cu1 N6 1.869(9) 2_746 ?
Cl1 Cu2 2.7451(18) 5_775 ?
Cl1 Cu2 2.7451(18) 6_575 ?
Cl1 Cu2 2.7451(18) 2_755 ?
V2 O3 1.885(11) 6_565 ?
V2 O7 2.094(14) 6_565 ?
V2 Mo4 2.807(10) . ?
V2 Mo1 2.807(5) . ?
V2 Mo1 2.807(5) 6_565 ?
V2 Mo2 3.082(10) . ?
Mo1 V1 2.9847(13) . ?
Mo2 O8 1.884(11) 6_565 ?
Mo2 O7 1.932(10) 6_565 ?
Mo2 O11 2.496(13) 6_565 ?
Mo3 O8 1.848(10) 6_565 ?
Mo3 O12 2.006(9) 2_756 ?
Mo3 O10 2.508(15) 2_756 ?
Mo3 V1 3.0251(14) . ?
Mo4 O6 1.860(10) 5_766 ?
Mo4 O6 1.860(10) 2_756 ?
Mo4 O3 1.942(9) 6_565 ?
Mo4 O10 2.495(14) 6_565 ?
O15 O15 1.20484(16) 2_756 ?
O15 V1 1.8115(2) . ?
V1 O15 1.8114(2) 2_756 ?
V1 O12 1.940(9) 2_756 ?
V1 O4 1.950(9) 2_756 ?
V1 Mo1 2.9847(13) 2_756 ?
V1 Mo3 3.0251(14) 2_756 ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
N4 C2 N1 N6 -0.6(13) . . . . ?
N4 C2 N1 Cu2 -178.2(8) . . . . ?
N3 C4 N2 N2 -0.6(12) . . . 6 ?
N3 C4 N2 Cu1 172.2(10) . . . . ?
N2 C4 N3 C4 0.9(19) . . . 6 ?
N2 C4 N3 Cu4 -170.9(10) . . . . ?
N1 C2 N4 C1 0.4(13) . . . . ?
N1 C2 N4 Cu3 -174.5(8) . . . . ?
N6 C1 N4 C2 0.0(14) . . . . ?
N6 C1 N4 Cu3 174.8(8) . . . . ?
N7 C3 N5 N5 -0.3(11) . . . 6 ?
N7 C3 N5 Cu2 -173.8(8) . . . 5_765 ?
N4 C1 N6 N1 -0.3(13) . . . . ?
N4 C1 N6 Cu1 -175.3(8) . . . 2_766 ?
C2 N1 N6 C1 0.5(12) . . . . ?
Cu2 N1 N6 C1 178.2(8) . . . . ?
C2 N1 N6 Cu1 175.8(8) . . . 2_766 ?
Cu2 N1 N6 Cu1 -6.6(13) . . . 2_766 ?
N5 C3 N7 C3 0.5(16) . . . 6 ?
N5 C3 N7 Cu4 175.3(8) . . . . ?
O10 O11 O10 P1 -43.2(8) 2_756 . . . ?
Mo1 O11 O10 P1 178.2(7) . . . . ?
Mo3 O11 O10 P1 -102.8(10) . . . . ?
Mo2 O11 O10 P1 104.4(11) . . . . ?
P1 O11 O10 O10 -45.3(4) . . . 6_565 ?
O10 O11 O10 O10 -88.5(7) 2_756 . . 6_565 ?
Mo1 O11 O10 O10 132.9(2) . . . 6_565 ?
Mo3 O11 O10 O10 -148.1(9) . . . 6_565 ?
Mo2 O11 O10 O10 59.1(9) . . . 6_565 ?
P1 O11 O10 O11 46.2(8) . . . 2_756 ?
O10 O11 O10 O11 3.0(13) 2_756 . . 2_756 ?
Mo1 O11 O10 O11 -135.5(7) . . . 2_756 ?
Mo3 O11 O10 O11 -56.6(14) . . . 2_756 ?
Mo2 O11 O10 O11 150.6(5) . . . 2_756 ?
P1 O11 O10 Mo1 -178.2(7) . . . . ?
O10 O11 O10 Mo1 138.6(7) 2_756 . . . ?
Mo3 O11 O10 Mo1 79.0(10) . . . . ?
Mo2 O11 O10 Mo1 -73.8(9) . . . . ?
P1 O11 O10 Mo4 -108.8(11) . . . . ?
O10 O11 O10 Mo4 -151.9(5) 2_756 . . . ?
Mo1 O11 O10 Mo4 69.5(10) . . . . ?
Mo3 O11 O10 Mo4 148.5(8) . . . . ?
Mo2 O11 O10 Mo4 -4.4(18) . . . . ?
P1 O11 O10 Mo3 106.8(10) . . . 2_756 ?
O10 O11 O10 Mo3 63.6(13) 2_756 . . 2_756 ?
Mo1 O11 O10 Mo3 -74.9(9) . . . 2_756 ?
Mo3 O11 O10 Mo3 4.0(17) . . . 2_756 ?
Mo2 O11 O10 Mo3 -148.8(7) . . . 2_756 ?
O11 O10 P1 O10 -120.3(6) . . . 6_565 ?
O11 O10 P1 O10 120.8(6) 2_756 . . 6_565 ?
Mo1 O10 P1 O10 -118.4(6) . . . 6_565 ?
Mo4 O10 P1 O10 1.6(11) . . . 6_565 ?
Mo3 O10 P1 O10 117.5(7) 2_756 . . 6_565 ?
O10 O10 P1 O10 180.000(4) 6_565 . . 2_756 ?
O11 O10 P1 O10 59.7(6) . . . 2_756 ?
O11 O10 P1 O10 -59.2(6) 2_756 . . 2_756 ?
Mo1 O10 P1 O10 61.6(6) . . . 2_756 ?
Mo4 O10 P1 O10 -178.4(11) . . . 2_756 ?
Mo3 O10 P1 O10 -62.5(7) 2_756 . . 2_756 ?
O10 O10 P1 O11 120.3(6) 6_565 . . . ?
O11 O10 P1 O11 -118.9(10) 2_756 . . . ?
Mo1 O10 P1 O11 1.9(7) . . . . ?
Mo4 O10 P1 O11 121.9(10) . . . . ?
Mo3 O10 P1 O11 -122.1(10) 2_756 . . . ?
O10 O10 P1 O11 -59.7(6) 6_565 . . 5_766 ?
O11 O10 P1 O11 180.001(2) . . . 5_766 ?
O11 O10 P1 O11 61.1(10) 2_756 . . 5_766 ?
Mo1 O10 P1 O11 -178.1(7) . . . 5_766 ?
Mo4 O10 P1 O11 -58.1(10) . . . 5_766 ?
Mo3 O10 P1 O11 57.9(10) 2_756 . . 5_766 ?
O10 O10 P1 O11 59.2(6) 6_565 . . 6_565 ?
O11 O10 P1 O11 -61.1(10) . . . 6_565 ?
O11 O10 P1 O11 180.000(6) 2_756 . . 6_565 ?
Mo1 O10 P1 O11 -59.2(10) . . . 6_565 ?
Mo4 O10 P1 O11 60.8(10) . . . 6_565 ?
Mo3 O10 P1 O11 176.8(7) 2_756 . . 6_565 ?
O10 O10 P1 O11 -120.8(6) 6_565 . . 2_756 ?
O11 O10 P1 O11 118.9(10) . . . 2_756 ?
Mo1 O10 P1 O11 120.8(10) . . . 2_756 ?
Mo4 O10 P1 O11 -119.2(10) . . . 2_756 ?
Mo3 O10 P1 O11 -3.2(7) 2_756 . . 2_756 ?
O10 O11 P1 O10 58.5(10) . . . 6_565 ?
O10 O11 P1 O10 180.000(1) 2_756 . . 6_565 ?
Mo1 O11 P1 O10 56.5(10) . . . 6_565 ?
Mo3 O11 P1 O10 -176.8(7) . . . 6_565 ?
Mo2 O11 P1 O10 -62.3(9) . . . 6_565 ?
O10 O11 P1 O10 -121.5(10) . . . 2_756 ?
Mo1 O11 P1 O10 -123.5(10) . . . 2_756 ?
Mo3 O11 P1 O10 3.2(7) . . . 2_756 ?
Mo2 O11 P1 O10 117.7(9) . . . 2_756 ?
O10 O11 P1 O10 179.997(3) . . . 5_766 ?
O10 O11 P1 O10 -58.5(10) 2_756 . . 5_766 ?
Mo1 O11 P1 O10 178.0(7) . . . 5_766 ?
Mo3 O11 P1 O10 -55.2(10) . . . 5_766 ?
Mo2 O11 P1 O10 59.2(9) . . . 5_766 ?
O10 O11 P1 O10 121.5(10) 2_756 . . . ?
Mo1 O11 P1 O10 -2.0(7) . . . . ?
Mo3 O11 P1 O10 124.8(10) . . . . ?
Mo2 O11 P1 O10 -120.8(9) . . . . ?
O10 O11 P1 O11 119.0(6) . . . 6_565 ?
O10 O11 P1 O11 -119.5(6) 2_756 . . 6_565 ?
Mo1 O11 P1 O11 117.0(6) . . . 6_565 ?
Mo3 O11 P1 O11 -116.2(6) . . . 6_565 ?
Mo2 O11 P1 O11 -1.8(10) . . . 6_565 ?
O10 O11 P1 O11 -61.0(6) . . . 2_756 ?
O10 O11 P1 O11 60.5(6) 2_756 . . 2_756 ?
Mo1 O11 P1 O11 -63.0(6) . . . 2_756 ?
Mo3 O11 P1 O11 63.8(6) . . . 2_756 ?
Mo2 O11 P1 O11 178.2(10) . . . 2_756 ?
C2 N1 Cu2 N5 31.1(17) . . . 5_765 ?
N6 N1 Cu2 N5 -146.0(9) . . . 5_765 ?
C2 N1 Cu2 Cl1 -147.5(10) . . . . ?
N6 N1 Cu2 Cl1 35.3(9) . . . . ?
C2 N4 Cu3 O13 118.3(17) . . . . ?
C1 N4 Cu3 O13 -55.3(17) . . . . ?
C4 N2 Cu1 N6 19(2) . . . 2_746 ?
N2 N2 Cu1 N6 -169.6(11) 6 . . 2_746 ?
Cu3 O13 V2 O3 133.2(7) . . . . ?
Cu3 O13 V2 O3 -133.2(7) . . . 6_565 ?
Cu3 O13 V2 O7 43.5(8) . . . . ?
Cu3 O13 V2 O7 -43.5(8) . . . 6_565 ?
Cu3 O13 V2 Mo4 180.000(1) . . . . ?
Cu3 O13 V2 Mo1 89.7(12) . . . . ?
Cu3 O13 V2 Mo1 -89.7(12) . . . 6_565 ?
Cu3 O13 V2 Mo2 0.000(2) . . . . ?
Mo1 O3 V2 O13 -113.4(17) . . . . ?
Mo4 O3 V2 O13 105.1(17) . . . . ?
Mo1 O3 V2 O3 137.4(3) . . . 6_565 ?
Mo4 O3 V2 O3 -4.1(8) . . . 6_565 ?
Mo1 O3 V2 O7 1.4(5) . . . . ?
Mo4 O3 V2 O7 -140.1(5) . . . . ?
Mo1 O3 V2 O7 62.4(8) . . . 6_565 ?
Mo4 O3 V2 O7 -79.1(8) . . . 6_565 ?
Mo1 O3 V2 Mo4 141.5(7) . . . . ?
Mo4 O3 V2 Mo1 -141.5(7) . . . . ?
Mo1 O3 V2 Mo1 107.9(5) . . . 6_565 ?
Mo4 O3 V2 Mo1 -33.6(6) . . . 6_565 ?
Mo1 O3 V2 Mo2 26.6(6) . . . . ?
Mo4 O3 V2 Mo2 -114.9(4) . . . . ?
Mo2 O7 Mo1 O2 152.1(10) . . . . ?
V2 O7 Mo1 O2 -101.3(5) . . . . ?
Mo2 O7 Mo1 O3 -105.1(11) . . . . ?
V2 O7 Mo1 O3 1.5(5) . . . . ?
Mo2 O7 Mo1 O4 51.3(11) . . . . ?
V2 O7 Mo1 O4 157.9(5) . . . . ?
Mo2 O7 Mo1 O12 -15(2) . . . . ?
V2 O7 Mo1 O12 91.4(10) . . . . ?
Mo2 O7 Mo1 O11 -9.1(10) . . . . ?
V2 O7 Mo1 O11 97.4(6) . . . . ?
Mo2 O7 Mo1 O10 -40.4(11) . . . . ?
V2 O7 Mo1 O10 66.1(5) . . . . ?
Mo2 O7 Mo1 V2 -106.6(13) . . . . ?
Mo2 O7 Mo1 V1 34.0(14) . . . . ?
V2 O7 Mo1 V1 140.6(3) . . . . ?
V2 O3 Mo1 O2 102.5(6) . . . . ?
Mo4 O3 Mo1 O2 -151.6(9) . . . . ?
V2 O3 Mo1 O7 -1.6(6) . . . . ?
Mo4 O3 Mo1 O7 104.3(9) . . . . ?
V2 O3 Mo1 O4 -93.8(10) . . . . ?
Mo4 O3 Mo1 O4 12.1(17) . . . . ?
V2 O3 Mo1 O12 -157.7(5) . . . . ?
Mo4 O3 Mo1 O12 -51.8(9) . . . . ?
V2 O3 Mo1 O11 -66.7(6) . . . . ?
Mo4 O3 Mo1 O11 39.2(9) . . . . ?
V2 O3 Mo1 O10 -96.8(6) . . . . ?
Mo4 O3 Mo1 O10 9.1(8) . . . . ?
Mo4 O3 Mo1 V2 105.9(11) . . . . ?
V2 O3 Mo1 V1 -141.3(3) . . . . ?
Mo4 O3 Mo1 V1 -35.5(11) . . . . ?
Mo3 O8 Mo2 O1 -161.4(12) 6_565 . . . ?
Mo3 O8 Mo2 O8 96.2(11) 6_565 . . 6_565 ?
Mo3 O8 Mo2 O7 -59.7(13) 6_565 . . 6_565 ?
Mo3 O8 Mo2 O7 10(2) 6_565 . . . ?
Mo3 O8 Mo2 O11 31.7(13) 6_565 . . . ?
Mo3 O8 Mo2 O11 0.9(11) 6_565 . . 6_565 ?
Mo3 O8 Mo2 V2 -40.7(15) 6_565 . . . ?
Mo4 O6 Mo3 O5 157.9(12) 5_766 . . . ?
Mo4 O6 Mo3 O8 -98.4(13) 5_766 . . 6_565 ?
Mo4 O6 Mo3 O12 56.0(12) 5_766 . . 2_756 ?
Mo4 O6 Mo3 O4 -5(2) 5_766 . . . ?
Mo4 O6 Mo3 O11 -33.0(13) 5_766 . . . ?
Mo4 O6 Mo3 O10 -4.0(11) 5_766 . . 2_756 ?
Mo4 O6 Mo3 V1 39.9(15) 5_766 . . . ?
Cu4 O9 Mo4 O6 46.7(4) 7_756 . . 5_766 ?
Cu4 O9 Mo4 O6 -46.7(4) 7_756 . . 2_756 ?
Cu4 O9 Mo4 O3 -136.9(3) 7_756 . . . ?
Cu4 O9 Mo4 O3 136.9(3) 7_756 . . 6_565 ?
Cu4 O9 Mo4 O10 -96(2) 7_756 . . . ?
Cu4 O9 Mo4 O10 96(2) 7_756 . . 6_565 ?
Cu4 O9 Mo4 V2 180.000(3) 7_756 . . . ?
Cu4 O15 V1 O15 171.9(2) . . . 2_756 ?
O15 O15 V1 O12 60.8(3) 2_756 . . 2_756 ?
Cu4 O15 V1 O12 -127.3(4) . . . 2_756 ?
O15 O15 V1 O12 -132.8(3) 2_756 . . . ?
Cu4 O15 V1 O12 39.1(3) . . . . ?
O15 O15 V1 O4 144.3(3) 2_756 . . 2_756 ?
Cu4 O15 V1 O4 -43.9(3) . . . 2_756 ?
O15 O15 V1 O4 -46.7(3) 2_756 . . . ?
Cu4 O15 V1 O4 125.1(4) . . . . ?
O15 O15 V1 Mo1 -95.15(3) 2_756 . . . ?
Cu4 O15 V1 Mo1 76.7(2) . . . . ?
O15 O15 V1 Mo1 107.02(3) 2_756 . . 2_756 ?
Cu4 O15 V1 Mo1 -81.1(2) . . . 2_756 ?
O15 O15 V1 Mo3 -174.33(2) 2_756 . . 2_756 ?
Cu4 O15 V1 Mo3 -2.5(2) . . . 2_756 ?
O15 O15 V1 Mo3 8.56(3) 2_756 . . . ?
Cu4 O15 V1 Mo3 -179.6(2) . . . . ?
